Yet again, new compounds found in systems with known binary phase diagrams. Synthesis, crystal and electronic structure of Nd<sub>3</sub>Bi<sub>7</sub> and Sm<sub>3</sub>Bi<sub>7</sub>.
Ovchinnikov, Alexander; Makongo, Julien P. A.; Bobev, Svilen; Chemical communications (Cambridge, England) 54 (2018) 7089–7092; doi:10.1039/c8cc02563k

data_7121800
_publ_section_title
;
 Yet again, new compounds found in systems with known binary phase
 diagrams. Synthesis, crystal and electronic structure of
 Nd<sub>3</sub>Bi<sub>7</sub> and Sm<sub>3</sub>Bi<sub>7</sub>.
;
_journal_issue                   51
_journal_name_full
'Chemical communications (Cambridge, England)'
_journal_page_first              7089
_journal_page_last               7092
_journal_paper_doi               10.1039/c8cc02563k
_journal_volume                  54
_journal_year                    2018
_chemical_formula_sum            'Bi7 Sm3'
_chemical_formula_weight         1913.91
_space_group_crystal_system      orthorhombic
_space_group_IT_number           71
_space_group_name_Hall           '-I 2 2'
_space_group_name_H-M_alt        'I m m m'
_symmetry_space_group_name_Hall  '-I 2 2'
_symmetry_space_group_name_H-M   'I m m m'
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2018-03-27 deposited with the CCDC.
2018-06-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.2762(8)
_cell_length_b                   15.050(3)
_cell_length_c                   19.034(4)
_cell_measurement_reflns_used    367
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      28.03
_cell_measurement_theta_min      3.45
_cell_volume                     1225.0(4)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0517
_diffrn_reflns_av_unetI/netI     0.0727
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            2557
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.420
_diffrn_reflns_theta_min         1.725
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    114.224
_exptl_absorpt_correction_T_max  0.048
_exptl_absorpt_correction_T_min  0.011
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    10.378
_exptl_crystal_description       block
_exptl_crystal_F_000             3068
_exptl_crystal_size_max          0.080
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.040
_refine_diff_density_max         3.039
_refine_diff_density_min         -4.512
_refine_diff_density_rms         0.864
_refine_ls_extinction_coef       0.000090(15)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.001
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     38
_refine_ls_number_reflns         931
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.001
_refine_ls_R_factor_all          0.0580
_refine_ls_R_factor_gt           0.0426
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0221P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0857
_refine_ls_wR_factor_ref         0.0924
_reflns_Friedel_coverage         0.000
_reflns_number_gt                701
_reflns_number_total             931
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c8cc02563k2.cif
_cod_data_source_block           shelx_CCDC1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Multi-scan' changed to
'multi-scan' according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 7121799--7121800.cif.
;
_cod_database_code               7121800
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.039
_shelx_estimated_absorpt_t_max   0.092
_shelx_res_checksum              41279